Carbohydrate Polymers 114 (2014) 537–545
Contents lists available at ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Preparation and properties of self-reinforced cellulose composite ﬁlms from Agave microﬁbrils using an ionic liquid K. Obi Reddy a,∗ , Jinming Zhang b , Jun Zhang b , A. Varada Rajulu c a b c
Department of Chemical Engineering Technology, Doornfontein Campus, University of Johannesburg, P.O. Box 17011, Johannesburg 2028, South Africa CAS Key Lab of Engineering Plastics, Institute of Chemistry, Chinese Academy of Sciences (CAS), Beijing, China Department of Physics, Osmania University, Hyderabad 500007, India
a r t i c l e
i n f o
Article history: Received 10 June 2014 Received in revised form 18 August 2014 Accepted 22 August 2014 Available online 30 August 2014 Keywords: Agave ﬁbers Cellulose microﬁbrils Ionic liquid Regenerated cellulose Spectroscopy Crystallinity
a b s t r a c t The applications of natural ﬁbers and their microﬁbrils are increasing rapidly due to their environment beneﬁts, speciﬁc strength properties and renewability. In the present work, we successfully extracted cellulose microﬁbrils from Agave natural ﬁbers by chemical method. The extracted microﬁbrils were characterized by chemical analysis. The cellulose microﬁbrils were found to dissolve in an ionic liquid 1-allyl-3-methylimidazolium chloride (AmimCl) to larger extent along with little quantity of undissolved microﬁbrils. Using this solution, the self-reinforced regenerated cellulose composite ﬁlms were prepared. The raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlms were characterized by FTIR, 13 C CP-MAS NMR, XRD, TGA and SEM techniques. The average tensile strength, modulus and elongation at break of the self-reinforced cellulose composite ﬁlms were found to be 135 MPa, 8150 MPa and 3.2%, respectively. The high values of tensile strength and modulus were attributed to the self-reinforcement of Agave ﬁbers in their generated matrix. These self-reinforced cellulose biodegradable composite ﬁlms prepared from renewable source can ﬁnd applications in packaging ﬁeld. © 2014 Elsevier Ltd. All rights reserved.
1. Introduction Recently, biomass-derived biodegradable ﬂexible and apparent ﬁlms, which are mostly based on cellulose, starch, protein, chitosan or their derivatives, have fascinated much attention because of their potential to substitute conventional petro-chemical products in many aspects (Biswas, Saha, Lawton, Shogren, & Willett, 2006; Pelissari, Grossmann, Yamashita, & Pineda, 2009; Yang et al., 2014). Cellulose is the world’s most common biopolymer and is measured as an almost never-ending source of raw material for the rising demand of environmentally gracious and biocompatible products (Eichhorn, 2011; Klemm et al., 2011). It has drawn much attention due to its unique properties such as low density simultaneously with high mechanical strength, low cost, renewability, biodegradability, good ﬁlm-forming performance, chemical stability and enormous of chemical derivations (Klemm, Heublein, Fink, & Bohn, 2005). There are several natural sources of cellulose; plants (major sources are wood and cotton), aerobic bacteria and some animals (tunicates). It has attracted more and more attention as a
∗ Corresponding author. Tel.: +27 846 606 269. E-mail addresses: [email protected]
, [email protected]
(K.O. Reddy). http://dx.doi.org/10.1016/j.carbpol.2014.08.054 0144-8617/© 2014 Elsevier Ltd. All rights reserved.
renewable resource for applications in the ﬁelds of material and energy (Eichhorn, 2011; Klemm et al., 2011). Cellulose is a linear polysaccharide composed of ␤-1-4-linked d-glucopyranose repeating units. Due to its many hydroxyl groups and to its tacticity, cellulose forms strong intra- and inter-molecular hydrogen bonds, giving rise to its three dimensional, supra-molecular and semicrystalline structures (Eichhorn, 2011). However, on description of the extensive bulky network linking hydrogen bonds and partially crystal structure, cellulose cannot be dissolved in water or most usual organic solvents (Soheilmoghaddam et al., 2014), which restricts its potential applications in forming processes. Several solvent systems have been developed to dissolve regenerated cellulose materials, such as NaOH/CS2 (Hyden, 1929), lithium chloride/N,N-dimethylacetamide (LiCl/DMAc) (McCormick, Callais, & Hutchinson, 1985), N-methylmorpholine-N-oxide (NMMO) (Fink, Weigel, Purz, & Ganster, 2001), phosphoric acid (Northolt et al., 2001), LiOH/urea and NaOH/urea (Cai & Zhang, 2005) and ionic liquids (Kosan, Michels, & Meister, 2008). However, ionic liquid (IL) has been gaining interest because of its potential to regenerate and chemically modify the cellulose over the other process (Swatloski, Spear, Holbrey, & Rogers, 2002; Zhu et al., 2006). Further, ionic liquids are characterized by excellent dissolubility, low toxicity, thermal stability, near zero volatility and recyclability
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
(Hameed, Guo, Tay, & Kazarian, 2011). Literature has indicated the availability of a variety of ionic liquid solvents for the production of regenerated cellulose from biomass (Cao, Li, Zhang, Zhang, & He, 2010; Casas et al., 2012; Fort et al., 2007; Jiang et al., 2011). Recent efforts have converted cellulose (obtained from biomass) to several forms like cellulose microﬁbrils, micro crystalline cellulose, nanocellulose, ﬁbrillated nanocellulose and nanocellulose whiskers with several end use applications (Eichhorn, 2011; Janardhnan & Sain, 2007; Maheswari, Reddy, Muzenda, Guduri, & Rajulu, 2012; Orts et al., 2005; Samir, Alloin, & Dufresne, 2005; Siro & Plackett, 2010; Taniguchi & Okamura, 1998). However, the consumption of energy to produce cellulose microﬁbrils is much lower than that of other cellulose derives. The microﬁbers are intended to be used in numerous applications varying from constituent part for plastic reinforcement, to gel forming food or cosmetic additives for their gelling, thickening properties in water and medical products (Lowys, Desbrieres, & Rinaudo, 2001; Mouro et al., 2003; Nakagaito & Yano, 2005). The natural Agave ﬁbers were selected in this work to extract cellulose microﬁbrils. Agave (also called century plant) belongs to the Agavaceae family of Agave americana L. species. Though this plant is native to Mexico and other parts of the Caribbean area, it is now cultivated worldwide as an ornamental plant (Msahli, Sakli, & Drean, 2006). It is widely used to make ropes and twines for agricultural purposes. In an earlier work, the authors reported the structural and physical properties of Agave ﬁbers (Reddy, Reddy, Zhang, Zhang, & Varada Rajulu, 2013). In this study, chemical treatments including acid-chlorite, alkaline and acid hydrolysis processes were used to produce cellulose microﬁbrils from Agave ﬁbers. These microﬁbrils were found to dissolve in the ionic liquid (1-allyl-3-methylimidazolium chloride) (AmimCl) to a larger extent with minor quantity of undissolved microﬁbrils. Using this solution, regenerated cellulose composite ﬁlms with self-reinforced microﬁbrils were prepared. The raw ﬁbers, extracted microﬁbers and regenerated cellulose composite ﬁlm were characterized by chemical analysis, FTIR, 13 CP-MAS NMR, Xray diffraction, morphology and thermogravimetric techniques and tensile testing. 2. Experimental 2.1. Materials Agave ﬁbers used in this study were extracted from the mature leaves of the plant by the usual water retting with beating process according to previous work (Reddy et al., 2013). After extraction, ﬁbers were cleaned with tap water to remove the unwanted materials from ﬁbers. Finally extracted ﬁbers were dried at room temperature for a week and stored in polyethylene bags. Acetic acid, ethanol, sodium bisulphite, sodium hydroxide pellets (Merck Chemicals), nitric acid, sodium chlorite and toluene (Sd-Fine Chemicals) chemicals used were of analytical grade. 2.2. Cellulose microﬁbrils extraction Extracted and chopped Agave ﬁbers were sieved through 250 mesh and dried at 105 ◦ C for 24 h. Then the ﬁbers were dewaxed by reﬂuxing with toluene–ethanol (2:1, v/v) for 6 h in a Soxhlet apparatus. The dewaxed ﬁber samples were then deligniﬁed with 0.7% sodium chlorite at 100 ◦ C for 2 h in acidic solution (pH 4–4.2 adjusted by 10% acetic acid) using a ﬁber to liquor ratio of 1:50. After being ﬁltered and extensively washed with 2% sodium bisulphite and distilled water, the residue was dried at 105 ◦ C in an oven until constant weight. The holocellulose was treated with 17.5% (w/v) NaOH solution at 20 ◦ C for 45 min, ﬁltered, washed
with 10% acetic acid, distilled water and ﬁnally dried at 105 ◦ C in an oven until constant weight. The extracted crude cellulose was treated with volume concentrations of 80% acetic acid −70% nitric acid taken in 10:1 ratio at 120 ◦ C for 20 min. After being cooled, it was then washed sequentially with 95% ethanol and distilled water to remove excess of acid mixture. Finally, the puriﬁed cellulose microﬁbrils were dried at 105 ◦ C in an oven until constant weight. The above procedure of extraction of cellulose microﬁbrils was adopted from Maheswari et al. (2012).
2.3. Chemical analysis The chemical composition of Agave raw ﬁbers and extracted cellulose microﬁbrils was determined using the standard TAPPI (Technical Association of the Pulp and Paper Associations) methods for different components, namely: T 204 cm-07 for extractives, T 203 cm-99 for ␣-cellulose, T 222 om-06 for lignin and T 211 om07 for ash content. The holocellulose was determined according to the method described by Wise, Murphy, and D’Addieco (1946). The hemicellulose fraction was calculated as the difference between the holocellulose and ␣-cellulose content. The percent contents of ␣-cellulose, hemicellulose and lignin were determined, and based on ﬁve samples the average and standard deviation values are reported.
2.4. Dissolution and regeneration of cellulose ﬁlm A distinct tentative process for preparation of regenerated cellulose ﬁlms with ionic liquid was as follows. First, the extracted cellulose microﬁbrils sample was added into a round bottom ﬂask containing AmimCl with a weight ratio of 4 wt% (cellulose microﬁbrils to AmimCl). The mixture of cellulose microﬁbrils/AmimCl was stirred continuously in an oil bath at 80 ◦ C with nitrogen atmosphere to form a solution having larger amounts of dissolved microﬁbrils and a little amount of undissolved microﬁbrils and then degassed. After that, the regenerated cellulose composite ﬁlms were prepared by casting the homogeneous mixture on glass plate. Then, the regenerated cellulose composite ﬁlms were soaked in deionized water and washed thoroughly to remove ionic liquid (no Cl− ions were detectable by the AgNO3 test). The obtained regenerated cellulose composite ﬁlms were dried in air for 48 h and stored in vacuum desiccators prior to characterization. These ﬁlms were found to be stable even after immersion in water for two days.
2.5. FTIR spectroscopy Fourier transform-infrared spectroscopy studies of raw ﬁbers, extracted cellulose microﬁbrils and the regenerated cellulose composite ﬁlms were carried out using a Smart iTR ATR Nicolet iS 10 FT-IR spectrophotometer. All the spectra were recorded in the 4000–500 cm−1 region with 32 scans in each case, at a resolution of 4 cm−1 .
2.6. NMR (CP-MAS) spectroscopy 13 C
cross-polarization magic angle spinning (CP-MAS) nuclear magnetic resonance (NMR) spectra of raw ﬁber, extracted cellulose microﬁbrils and the regenerated cellulose composite ﬁlms were run on a Bruker DSX 300 MHz solid-state NMR spectrometer. The operating frequency for 13 C nuclei was ﬁxed at 75.46 MHz, and the samples ﬁlled in 5 mm rotor were spun at a rate of 5 kHz at room temperature.
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
2.7. X-ray diffraction analysis Wide-angle X-ray diffractograms of raw ﬁbers, extracted cellulose microﬁbrils and the regenerated cellulose composite ﬁlms were recorded on a Rigaku Ultima IV X-ray diffractometer. The system has a rotating anode generator with a copper target and a wide-angle powder goniometer. The generator was operated ˚ and at 40 kV power using ﬁltered Cu K␣ radiation ( = 1.5406 A) 30 mA, and the samples were scanned in the 2 range of 5–50◦ . The crystallinity index (CrI) was calculated by Segal’s method (Segal, Creely, Martin, & Conrad, 1959) using the following equation: CrI =
Ihkl − Iam Ihkl
where Ihkl is the intensity of diffraction maximum of crystalline regions [I200 (22.8◦ ) in cellulose I; I200 (21.9◦ ) in cellulose II], while Iam is the intensity value for the amorphous cellulose close to 17.3◦ (Sèbe, Ham-Pichavant, Ibarboure, Kofﬁ, & Tingaut, 2012). 2.8. Thermogravimetric analysis The thermal stability of Agave raw ﬁbers, extracted cellulose micro ﬁbrils and regenerated cellulose composite ﬁlms were established using a thermogravimetric analyzer (Perkin Elmer TGA-7). The amount of sample for each measurement was about 10 mg. All the measurements were performed under a nitrogen atmosphere with a gas ﬂow of 100 mL/min and heated from 50 to 600 ◦ C at a rate of 10 ◦ C/min. 2.9. Morphology Scanning electron microscope (JEOL JSM 820) was used to study the morphology of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm. The samples were gold coated prior to recording the micrographs. The acceleration voltage was set at 5 kV. 2.10. Tensile testing An Universal testing machine (Instron 3369) with a 10 kN loaded cell was used to determine the tensile strength, Young’s modulus and elongation at break of the ﬁlms at a constant extension speed of 5 mm/min. regenerated cellulose composite ﬁlms were cut into rectangular shape with a length of 100 mm and a width of 10 mm, and were then clipped by two clamps on instrument. Five specimens were used for tensile test and the average values of tensile properties were reported. The tests were conducted at a temperature of 30 ◦ C and relative humidity of 70%. 3. Results and discussion 3.1. Chemical analysis The primary work concerned in the present research was to extract ﬁbers from Agave leaves, subsequently convert them into cellulose microﬁbrils and characterize them. It was also planned to dissolve the microﬁbrils in an ionic liquid and make regenerated cellulose ﬁlm. According to chemical analysis results, raw ﬁbers contained 71.65% of ␣-cellulose, 22.24% of hemicellulose and 6.09% of lignin. The extracted cellulose microﬁbrils contained ␣-cellulose, hemicellulose and lignin contents in 93.3, 2.35 and 3.69%, respectively. From the chemical analysis, it is evident that the ␣-cellulose content increased while the lignin and hemicellulose decreased in the case of microﬁbrils when compared to the raw ﬁbers. This may be attributed to the effect of chemicals that were used during the cellulose microﬁbrils extraction process. This proves that during
the acidiﬁed sodium chlorite, sodium hydroxide and acid hydrolysis treatments signiﬁcant breakdown of the ligno-cellulosic structure took place resulting in the hydrolysis of hemicellulose fraction and depolymerization of lignin. In order to further probe this, we also carried out FTIR and 13 C NMR (CP-MAS) analyses. 3.2. FTIR spectra analysis The FTIR spectra of the Agave raw ﬁber, cellulose microﬁbrils and the regenerated cellulose composite ﬁlm are shown in Fig. 1. From Fig. 1, it is evident that, the three spectra had well deﬁned common bands at 3333, 2917, 1427, 1369, 1316, 1159, 1101, 1052, 1030 and 897 cm−1 corresponding to cellulose (Liu et al., 2006; Sain & Panthapulakkal, 2006; Maheswari et al., 2012; Reddy et al., 2013). Further, an additional common band at around 1626 cm−1 was found in all the three cases that was attributed to the bending mode of the absorbed water (Sain & Panthapulakkal, 2006). However, in the case of raw ﬁbers, additional bands at around 1731, 1509, 1461 and 1243 cm−1 were also present that were attributed to hemicellulose and lignin (Reddy, Guduri, & Rajulu, 2009; Maheswari et al., 2012; Reddy et al., 2013). The intensity of these bands decreased in the extracted cellulose microﬁbrils, because of the most of removal of hemicellulose and lignin by chemical treatments in cellulose extraction process. The similarity of FTIR spectra of the original cellulose microﬁbrils and regenerated cellulose composite ﬁlm indicates that there was no effect of ionic liquid in cellulose structure. However, the intensity of the O H stretching of cellulose microﬁbrils band was found to be very low as compared to the regenerated cellulose due to splitting of hydrogen bonds in the cellulose (Zhang, Wu, Zhang, & He, 2005). Therefore, it could be concluded that the regenerated cellulose was without any derivatization during the dissolution and regeneration processes. 3.3.
CP-MAS NMR spectra analysis
The 13 C CP-MAS (cross-polarization magic angle spinning) NMR spectra for the raw ﬁber, cellulose microﬁbrils and regenerated cellulose composite ﬁlm are shown in Fig. 2. The spectrum of raw ﬁber mainly shows the corresponding signals for the cellulose, hemicellulose, and lignin. The entire noticeable peaks of the cellulose carbon atoms occurred in the range of 60 to 110 ppm (Maheswari et al., 2012). The most prominent peaks of raw ﬁber were the superimposed C-2, C-3 and C-5 signals at 73.1–75.9 ppm, and other important features were C-1 (105.7 ppm), C-4 (89.7 ppm) and C-6 (65.8 ppm), while the peak at 84.4 ppm is due to the disordered C-4 carbon of cellulose (Reddy et al., 2009). The carbon peaks of the hemicellulose are expected at 103 ppm (C-1), 84 ppm (C-4), 72–75 ppm (C-2 and C-3) and 65 ppm (C-5), but the strong cellulose peaks overlapped these peaks (Maheswari et al., 2012). The spectrum of raw ﬁber shows a sharp moderate peak at 21.5 ppm, and a broad peak at 172.9 ppm. These peaks were attributed to the methyl and carboxylic carbons of acetyl groups in hemicellulose (Reddy et al., 2009). The lignin peaks appeared between 110 and 160 ppm, which were assigned to different aromatic carbons of lignin (Capanema, Balakshin, & Kadla, 2004; Nadji et al., 2009). In addition, the peak between 10 and 40 ppm was attributed to the methyl and alkyl carbons (including acetyl groups in hemicellulose), while the peak at 56.6 ppm was attributed to methoxyl ( OCH3 ) and carbonyl groups, respectively, in lignin (Reddy et al., 2009). The extracted cellulose microﬁbrils (form raw ﬁber) spectrum (Fig. 2) indicated the disappearance of peaks at 110–160 ppm, 56.6 ppm and 10–40 ppm of lignin, as well as 21.5 and 172.9 ppm of hemicellulose indicating that most of hemicellulose and lignin were successfully removed as a result of the different chemical treatments by cellulose extraction
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
Fig. 1. FTIR spectra of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm.
process. While the other (cellulose) peaks, i.e., those appeared in the region 60–110 ppm almost remained the same. The NMR spectrum of regenerated cellulose composite ﬁlm is also shown in Fig. 2. The inconsequential features of the spectrum of the deshielding of its chemical shift were observed which further indicates that there was no effect of ionic liquid in cellulose structure of regenerated ﬁlms.
Fig. 2. NMR spectra of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm.
3.4. X-ray diffraction analysis The crystallinity of the extracted cellulose was investigated by using XRD. Certainly, cellulose has a crystalline structure with respect to hemicellulose and lignin, which are amorphous in nature. More speciﬁcally, cellulose has a crystalline structure due to the hydrogen bond interactions and van der Waals forces between adjacent macromolecules (Zhang & Lynd, 2004). X-ray diffraction (XRD) analysis was used to evaluate the crystallinity of the raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm. Though all the samples were semi-crystalline, the crystallinity was somewhat different among them. The XRD patterns of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm are shown in Fig. 3. The X-ray diffractogram of raw ﬁber shows a strong crystalline peak at 22.8◦ for (2 0 0) crystal plane, a small peak at 34.6◦ for (0 0 4) crystal plane, and a broad peak at 16.0◦ overlapped by 15.1◦ (1 −1 0) crystal plane and 16.8◦ (1 1 0) crystal plane, which indicate a cellulose I crystalline structure of raw ﬁber (Oh et al., 2005). In the extracted cellulose microﬁbrils (Fig. 3), a notably unique diffraction pattern assigned as the mixture of cellulose I and II was observed. Except the peaks of cellulose I, new peaks at 2 = 12.4◦ (1 −1 0), 20.1◦ (1 1 0) and 21.9◦ (2 0 0) appeared to indicate the formation of cellulose II. That is to say, the native cellulose (cellulose I) was partially transformed into cellulose II through the chemical extraction process of cellulose microﬁbrils. The diffractogram of the regenerated cellulose composite ﬁlm indicated that the main diffraction peak appeared at 20–22◦ (cellulose II), with relatively low intensity, and the peak shape was broad. Further the subsidiary diffraction peaks (12.4◦ , 15.1◦ , 16.8◦ and 34.6◦ ) were almost nonexistent. All of the phenomena indicated that the areas of crystal region became small, and the regenerated cellulose ﬁlm mainly attained an amorphous structure. The calculated crystallinity index (CrI) values of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm were found to be 57.2, 64.4 and 55.9%, respectively. The crystallinity index of extracted cellulose microﬁbrils was found to be higher than the raw ﬁber and regenerated cellulose composite ﬁlm due to the removal of non-cellulosic materials. During the hydrolysis process, hydronium ions can penetrate the more accessible amorphous regions of cellulose to allow the hydrolytic cleavage of glycosidic bonds. As a result, the raw ﬁbers eventually release individual crystallites and these monocrystals are
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
Fig. 3. X-Ray diffractograms of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm.
realigned, which improve the cellulose crystallinity (Johar, Ahmad, & Dufresne, 2012). The lower crystallinity in the regenerated cellulose composite ﬁlm (Lee, Doherty, Linhardt, & Dordick, 2009) was probably caused by the rapid depolymerization of cellulose in the dissolving process (Zhang et al., 2005). 3.5. Thermogravimetric analysis Thermogravimetric analysis (TGA) was deliberate to access the thermal stability of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm and the corresponding primary thermograms are shown in Fig. 4. The samples decomposition is exhibited in two stages, indicating the presence of three different
constituents (Yang, Yan, Chen, Lee, & Zheng, 2007). The ﬁrst decomposition stage was found in 250–350 ◦ C temperature range for raw ﬁber. During this stage, thermal depolymerization of hemicelluloses and some fraction of lignin resulted besides destruction of crystalline regions of cellulose. These were then slowly transformed into CO2 and volatile hydrocarbons. The weight loss in this temperature range was found to be 25%. The second degradation stage occurred in the range of 350–440 ◦ C for raw ﬁber. The weight loss over these temperature ranges was found to be 56.5%. During this stage cellulose was almost completely burnt because of the continuing thermal oxidative degradation of the char produced. However, in the extracted cellulose microﬁbrils, the ﬁrst degradation stage started in the region 280–370 ◦ C and the corresponding
Fig. 4. Primary thermograms of raw ﬁber, extracted cellulose microﬁbrils and regenerated cellulose composite ﬁlm.
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
weight loss in this temperature range was found to be 39%. These results clearly illustrate that the thermal stability of the extracted cellulose microﬁbrils was higher than that of the raw ﬁbers. This was attributed to the removal of hemicellulose and lignin from the raw ﬁbers on several chemical treatments. The second degradation stage started in the region 370–440 ◦ C and the weight loss in this temperature was found to be 70%. Further for the regenerated cellulose composite ﬁlm, the ﬁrst and second degradation stages occurred in the regions 240–330 and 340–470 ◦ C, respectively, with the corresponding weight loss of 23.6 and 50.8%, respectively. The lower thermal stability of regenerated cellulose composite ﬁlm compared to the raw ﬁber and extracted cellulose microﬁbrils was due to the low crystallinity of regenerated cellulose. Similar results were reported during the dissolution of cellulose in ionic liquid (Swatloski et al., 2002; Liu et al., 2007; Li, Wu, Chen, Liu, & Sun, 2011). However, the char content of the regenerated cellulose composite was found to be higher than that of raw ﬁber and microﬁbrils. 3.6. Surface morphology The morphology of raw century ﬁbers and extracted cellulose microﬁbrils was studied using scanning electron microscope. Fig. 5 reveals the morphological changes between the raw Agave ﬁbers and extracted cellulose microﬁbrils. The micrographs of raw century ﬁber surface shown in Fig. 5a and b reveal that the impurities were localized on the surface. Generally most of natural cellulose ﬁbers are with multi cellular structure and then composed of cellulose surrounded and cemented together with lignin and hemicelluloses. In our earlier studies, the chemical composition and structural characterization of raw century (Agave) ﬁbers were already reported (Reddy et al., 2013). Following the completion of several chemical treatments, most of the lignin and hemicellulose were removed to large extent and the cellulose microﬁbrils were separated from the raw ﬁbers (from Fig. 5c and d). The micrographs also indicate a highly ﬁbrous network-like structure consisting of
Fig. 6. Scanning electron micrograph of regenerated cellulose composite ﬁlm surface.
cellulose microﬁbrils. It is clear from the micrographs that the range of diameter of the microﬁbrils was about 8–14 m, which was lower than that of diameter of raw ﬁbers (0.21 mm). In addition, some structures of bundled ﬁbers are still detectable (Fig. 5c). At higher magniﬁcation (Fig. 5d), microﬁbrils appear to have a clean and rough surface. The morphological changes in the ﬁber surface were recognized to the removal of the hemicelluloses and lignin by chemical treatments. As well, the morphology of produced regenerated cellulose composite ﬁlm was analyzed by scanning electron microscopy (SEM), and the corresponding micrograph is shown in Fig. 6. It can be seen
Fig. 5. Scanning electron micrographs raw ﬁber surfaces ((a) and (b)) and extracted cellulose microﬁbrils surface ((c) and (d)) at different magniﬁcations.
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
Table 1 Comparison of tensile properties of regenerated cellulose composite ﬁlm with various biopolymer ﬁlms. Biopolymer ﬁlms
Film preparation method
Tensile strength (MPa)
Tensile modulus (MPa)
Elongation at break (%)
Polylactic acid (PLA) Polyvinyl alcohol (PVA) Polypropylene carbonate (PPC) Polyhydroxybutyrate (PHBV) Banana starch (BS) Cassava starch (CS) Sweet potato starch (SPS) Chitosan (CH) Regenerated cellulose (RC)
Solution casting Solution casting Solution casting Solution casting Solution casting Solution casting Solution casting Solution casting Solution casting
16.8 83 12.8 28.9 5.01 2.56 3.72 8.4 135
1152 1900 823 3570 46.86 30.27 106.01 134.6 8150
402 45 821 10.2 14.30 43.45 33.83 19.6 3.2
Ashok et al. (2014) Zhang et al. (2003) Feng et al. (2014) Cyras et al. (2007) Torres et al. (2011) Torres et al. (2011) Torres et al. (2011) Pereda et al. (2014) Present work
conﬁrms the formation of all cellulose composite ﬁlm. The visible fairly transparency and high ﬂexibility of the regenerated cellulose casting ﬁlm is demonstrated in Fig. 7. 3.7. Tensile properties
Fig. 7. Photograph of the regenerated cellulose composite ﬁlm taken before a plant.
from SEM micrograph that regenerated cellulose composite ﬁlm exhibited cellulose continuous phase along with cellulose microﬁbrils as the discontinuous phase. The presence of microﬁbrils in the composite ﬁlm can be visualized in the micrograph. This further
To evaluate the tensile properties of the regenerated cellulose composite ﬁlm, the corresponding stress–strain curves of ﬁve ﬁlm specimens are shown in Fig. 8. From Fig. 8, the regenerated cellulose ﬁlm showed a behavior with stress increasing rapidly at small strains and more slowly after the yield point. The average tensile strength, Young’s modulus and %elongation at break of the regenerated cellulose composite ﬁlm were found to be 135 ± 8 MPa, 8150 ± 257 MPa and 3.2 ± 0.2%, respectively, which are higher than for the ﬁlms made using cotton linters. In comparison, the tensile strength for the regenerated cellulose ﬁlms obtained with AmimCl was higher than that of the largely used commercial polyoleﬁn ﬁlms, such as polypropylene (PP) and polyethylene (PE) with tensile strength in the range of 20–40 MPa (Ding, 1995). The tensile properties of regenerated cellulose composite ﬁlm were compared with those of other biopolymer ﬁlms (Ashok et al., 2014; Cyras, Commisso, Mauri, & Vazquez, 2007; Feng et al., 2014; Pereda, Dufresne, Aranguren, & Marcovich, 2014; Torres, Troncoso, Torres, Díaz, & Amaya, 2011; Zhang et al., 2003) and are presented in Table 1. From this table, it can be observed that the tensile strength and tensile modulus of regenerated cellulose composite
Fig. 8. Stress–strain curve of ﬁve regenerated cellulose composite ﬁlm specimens.
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545
ﬁlm from Agave ﬁber were higher than other biopolymer ﬁlms, while the elongation at break was lower than other biopolymer ﬁlms. The increase in tensile strength and modulus of regenerated cellulose composite ﬁlms could be due to the covalent bonding of soluble cellulose with insoluble cellulose microﬁbrils, which lead to an increase in the stiffness, which usually led to a decrease in the deformation capability of the regenerated cellulose composite ﬁlms. 4. Conclusion Agave leaf ﬁbers are interesting alternative as cellulose source for several applications. This material is renewable and hugely available in many regions of the world. An effective and convenient chemical process was used to extract the cellulose microﬁbrils from Agave ﬁbers. The Agave microﬁbrils were found to dissolve in the ionic liquid AmimCl to a very large extent with little amount of undissolved microﬁbrils. Using the solution, the regenerated cellulose composite ﬁlms with self-reinforced microﬁbrils were prepared. The chemical analysis results showed that extracted cellulose microﬁbrils had higher cellulose content and lower hemicellulose and lignin contents than the raw ﬁbers. The results derived from the FTIR and NMR analyses conﬁrmed that both lignin and most of the hemicellulose were removed during the chemical process. X-ray diffraction results conﬁrmed the partial transition from cellulose I to II during the preparation of cellulose microﬁbrils. The regenerated cellulose composite ﬁlms had lower crystallinity. All samples revealed two-step decomposition behavior with the degradation temperatures of 250 ◦ C for raw ﬁbers, 280 ◦ C for cellulose microﬁbrils and 240 ◦ C for regenerated cellulose composite ﬁlm suggesting an enhanced thermal stability of cellulose microﬁbrils. The SEM results illustrated that most of the microﬁbrils extracted from century ﬁber had diameters in the range of 8–14 m. The micrograph of the surface of the regenerated cellulose composite ﬁlm displayed the presence of reinforced microﬁbrils. Fairly optically transparent ﬁlms were obtained by casting, which could be potentially used as optical components for advanced applications. The notable properties of the regenerated cellulose ﬁlms are promising for applications in transparent biodegradable packaging purpose as a substitute for PP and PE. In general, regenerated cellulose ﬁlms due to their excellent tensile properties should have a promising impact in food packaging over the coming years. This paper demonstrated that the Agave ﬁbers under study can be potentially used as raw material for the production of regenerated cellulose ﬁlms. Acknowledgements The author KOR sincerely acknowledges the Faculty of Engineering and Built Environment, University of Johannesburg, South Africa, for the award of Postdoctoral Research Fellowship. The author AVR thanks the Council of Scientiﬁc and Industrial Research of India for the award of an Emeritus Scientist, Scheme [21(0842)11/EMR-II dt:10-05-2011]. References Ashok, B., Naresh, S., Reddy, K. O., Madhukar, K., Cai, J., Zhang, L., et al. (2014). Tensile and thermal properties of poly(lactic acid)/eggshell powder composite ﬁlms. International Journal of Polymer Analysis and Characterization, 19(3), 245–255. Biswas, A., Saha, B. C., Lawton, J. W., Shogren, R. L., & Willett, J. L. (2006). Process for obtaining cellulose acetate from agricultural by-products. Carbohydrate Polymers, 64(1), 134–137. Cai, J., & Zhang, L. (2005). Rapid dissolution of cellulose in LiOH/urea and NaOH/urea aqueous solutions. Macromolecular Bioscience, 5(6), 539–548. Cao, Y., Li, H., Zhang, Y., Zhang, J., & He, J. (2010). Structure and properties of novel regenerated cellulose ﬁlms prepared from cornhusk cellulose in room temperature ionic liquids. Journal of Applied Polymer Science, 116(1), 547–554.
Capanema, E. A., Balakshin, M. Y., & Kadla, J. F. (2004). A comprehensive approach for quantitative lignin characterization by NMR spectroscopy. Journal of Agricultural and Food Chemistry, 52(7), 1850–1860. Casas, A., Palomar, J., Alonso, M. V., Oliet, M., Omar, S., & Rodriguez, F. (2012). Comparison of lignin and cellulose solubilities in ionic liquids by COSMO-RS analysis and experimental validation. Industrial Crops and Products, 37(1), 155–163. Cyras, V. P., Commisso, M. S., Mauri, A. N., & Vazquez, A. (2007). Biodegradable double-layer ﬁlms based on biological resources: Polyhydroxybutyrate and cellulose. Journal of Applied Polymer Science, 106(2), 749–756. Ding, H. (1995). Handbook of plastic industry. Beijing: Chemical Industry Press. Eichhorn, S. J. (2011). Cellulose nanowhiskers: Promising materials for advanced applications. Soft Matter, 7(2), 303–315. Fink, H. P., Weigel, P., Purz, H. J., & Ganster, J. (2001). Structure formation of regenerated cellulose materials from NMMO-solutions. Progress in Polymer Science, 26(9), 1473–1524. Feng, Y., Ashok, B., Madhukar, K., Zhang, J., Zhang, J., Reddy, K. O., et al. (2014). Preparation and characterization of polypropylene carbonate bio-ﬁller (egg shell powder) composite ﬁlms. International Journal of Polymer Analysis and Characterization, http://dx.doi.org/10.1080/1023666X.2014.953747 (in press) Fort, D. A., Remsing, R. C., Swatloski, R. P., Moyna, P., Moyna, G., & Rogers, R. D. (2007). Can ionic liquids dissolve wood? Processing and analysis of lignocellulosic materials with 1-n-butyl-3-methylimidazolium chloride. Green Chemistry, 9(1), 63–69. Hameed, N., Guo, Q., Tay, F. H., & Kazarian, S. G. (2011). Blends of cellulose and poly (3-hydroxybutyrate-co-3-hydroxyvalerate) prepared from the ionic liquid 1-butyl-3-methylimidazolium chloride. Carbohydrate Polymers, 86(1), 94–104. Hyden, W. L. (1929). Manufacture and properties of regenerated cellulose ﬁlms. Industrial & Engineering Chemistry, 21(5), 405–410. Janardhnan, S., & Sain, M. M. (2007). Isolation of cellulose microﬁbrils—An enzymatic approach. BioResources, 1(2), 176–188. Jiang, M., Zhao, M., Zhou, Z., Huang, T., Chen, X., & Wang, Y. (2011). Isolation of cellulose with ionic liquid from steam exploded rice straw. Industrial Crops and Products, 33(3), 734–738. Johar, N., Ahmad, I., & Dufresne, A. (2012). Extraction, preparation and characterization of cellulose ﬁbres and nanocrystals from rice husk. Industrial Crops and Products, 37(1), 93–99. Klemm, D., Heublein, B., Fink, H. P., & Bohn, A. (2005). Cellulose: Fascinating biopolymer and sustainable raw material. Angewandte Chemie International Edition, 44(22), 3358–3393. Klemm, D., Kramer, F., Moritz, S., Lindström, T., Ankerfors, M., Gray, D., et al. (2011). Nanocelluloses: A new family of nature-based materials. Angewandte Chemie International Edition, 50(24), 5438–5466. Kosan, B., Michels, C., & Meister, F. (2008). Dissolution and forming of cellulose with ionic liquids. Cellulose, 15(1), 59–66. Lee, S. H., Doherty, T. V., Linhardt, R. J., & Dordick, J. S. (2009). Ionic liquid-mediated selective extraction of lignin from wood leading to enhanced enzymatic cellulose hydrolysis. Biotechnology and Bioengineering, 102(5), 1368–1376. Li, W., Wu, L., Chen, D., Liu, C., & Sun, R. (2011). DMAP-catalyzed phthalylation of cellulose with phthalic anhydride in [bmim] Cl. BioResources, 6(3), 2375–2385. Liu, C. F., Sun, R. C., Zhang, A. P., Ren, J. L., Wang, X. A., Qin, M. H., et al. (2007). Homogeneous modiﬁcation of sugarcane bagasse cellulose with succinic anhydride using a ionic liquid as reaction medium. Carbohydrate Research, 342(7), 919–926. Liu, C. F., Xu, F., Sun, J. X., Ren, J. L., Curling, S., Sun, R. C., et al. (2006). Physicochemical characterization of cellulose from perennial ryegrass leaves (Lolium perenne). Carbohydrate Research, 341(16), 2677–2687. Lowys, M. P., Desbrieres, J., & Rinaudo, M. (2001). Rheological characterization of cellulosic microﬁbril suspensions. Role of polymeric additives. Food Hydrocolloids, 15(1), 25–32. Maheswari, C. U., Reddy, K. O., Muzenda, E., Guduri, B. R., & Rajulu, A. V. (2012). Extraction and characterization of cellulose microﬁbrils from agricultural residue—Cocos nucifera L. Biomass and Bioenergy, 46, 555–563. McCormick, C. L., Callais, P. A., & Hutchinson, B. H., Jr. (1985). Solution studies of cellulose in lithium chloride and N,N-dimethylacetamide. Macromolecules, 18(12), 2394–2401. Mouro, C. R., Bouchet, B., Pontoire, B., Robert, P., Mazoyer, J., & Buléon, A. (2003). Structural features and potential texturising properties of lemon and maize cellulose microﬁbrils. Carbohydrate Polymers, 53(3), 241–252. Msahli, S., Sakli, F., & Drean, J. Y. (2006). Study of textile potential of ﬁbers extracted from Tunisian Agave americana L. AUTEX Research Journal, 6(1), 9–13. Nadji, H., Diouf, P. N., Benaboura, A., Bedard, Y., Riedl, B., & Stevanovic, T. (2009). Comparative study of lignins isolated from Alfa grass (Stipa tenacissima L.). Bioresource Technology, 100(14), 3585–3592. Nakagaito, A. N., & Yano, H. (2005). Novel high-strength biocomposites based on microﬁbrillated cellulose having nano-order-unit web-like network structure. Applied Physics A, 80(1), 155–159. Northolt, M. G., Boerstoel, H., Maatman, H., Huisman, R., Veurink, J., & Elzerman, H. (2001). The structure and properties of cellulose ﬁbres spun from an anisotropic phosphoric acid solution. Polymer, 42(19), 8249–8264. Oh, S. Y., Yoo, D. I., Shin, Y., Kim, H. C., Kim, H. Y., Chung, Y. S., et al. (2005). Crystalline structure analysis of cellulose treated with sodium hydroxide and carbon dioxide by means of X-ray diffraction and FTIR spectroscopy. Carbohydrate Research, 340(15), 2376–2391. Orts, W. J., Shey, J., Imam, S. H., Glenn, G. M., Guttman, M. E., & Revol, J. F. (2005). Application of cellulose microﬁbrils in polymer nanocomposites. Journal of Polymers and the Environment, 13(4), 301–306.
K.O. Reddy et al. / Carbohydrate Polymers 114 (2014) 537–545 Pelissari, F. M., Grossmann, M. V., Yamashita, F., & Pineda, E. A. G. (2009). Antimicrobial, mechanical, and barrier properties of cassava starch–chitosan ﬁlms incorporated with oregano essential oil. Journal of Agricultural and Food Chemistry, 57(16), 7499–7504. Pereda, M., Dufresne, A., Aranguren, M. I., & Marcovich, N. E. (2014). Polyelectrolyte ﬁlms based on chitosan/olive oil and reinforced with cellulose nanocrystals. Carbohydrate Polymers, 101, 1018–1026. Reddy, K. O., Guduri, B. R., & Rajulu, A. V. (2009). Structural characterization and tensile properties of borassus fruit ﬁbers. Journal of Applied Polymer Science, 114(1), 603–611. Reddy, K. O., Reddy, K. R. N., Zhang, J., Zhang, J., & Varada Rajulu, A. (2013). Effect of alkali treatment on the properties of Century ﬁber. Journal of Natural Fibers, 10(3), 282–296. Sain, M., & Panthapulakkal, S. (2006). Bioprocess preparation of wheat straw ﬁbers and their characterization. Industrial Crops and Products, 23(1), 1–8. Samir, M. A. S. A., Alloin, F., & Dufresne, A. (2005). Review of recent research into cellulosic whiskers, their properties and their application in nanocomposite ﬁeld. Biomacromolecules, 6(2), 612–626. Sèbe, G., Ham-Pichavant, F., Ibarboure, E., Kofﬁ, A. L. C., & Tingaut, P. (2012). Supramolecular structure characterization of cellulose II nanowhiskers produced by acid hydrolysis of cellulose I substrates. Biomacromolecules, 13(2), 570–578. Segal, L. G. J. M. A., Creely, J. J., Martin, A. E., & Conrad, C. M. (1959). An empirical method for estimating the degree of crystallinity of native cellulose using the X-ray diffractometer. Textile Research Journal, 29(10), 786–794. Siró, I., & Plackett, D. (2010). Microﬁbrillated cellulose and new nanocomposite materials: A review. Cellulose, 17(3), 459–494. Soheilmoghaddam, M., Wahit, M. U., Tuck Whye, W., Ibrahim Akos, N., Heidar Pour, R., & Ali Yussuf, A. (2014). Bionanocomposites of regenerated cellulose/zeolite
prepared using environmentally benign ionic liquid solvent. Carbohydrate Polymers, 106, 326–334. Swatloski, R. P., Spear, S. K., Holbrey, J. D., & Rogers, R. D. (2002). Dissolution of cellose with ionic liquids. Journal of the American Chemical Society, 124(18), 4974–4975. Taniguchi, T., & Okamura, K. (1998). New ﬁlms produced from microﬁbrillated natural ﬁbres. Polymer International, 47(3), 291–294. Torres, F. G., Troncoso, O. P., Torres, C., Díaz, D. A., & Amaya, E. (2011). Biodegradability and mechanical properties of starch ﬁlms from Andean crops. International Journal of Biological Macromolecules, 48(4), 603–606. Wise, L. E., Murphy, M., & D’Addieco, A. A. (1946). Chlorite holocellulose: Its fractionation and bearing on summative wood analysis and on studies on the hemicellulose. Paper Trade Journal, 122(2), 35–43. Yang, D., Peng, X., Zhong, L., Cao, X., Chen, W., Zhang, X., et al. (2014). Green ﬁlms from renewable resources: Properties of epoxidized soybean oil plasticized ethyl cellulose ﬁlms. Carbohydrate Polymers, 103, 198–206. Yang, H., Yan, R., Chen, H., Lee, D. H., & Zheng, C. (2007). Characteristics of hemicellulose, cellulose and lignin pyrolysis. Fuel, 86(12), 1781–1788. Zhang, H., Wu, J., Zhang, J., & He, J. (2005). 1-Allyl-3-methylimidazolium chloride room temperature ionic liquid: A new and powerful nonderivatizing solvent for cellulose. Macromolecules, 38(20), 8272–8277. Zhang, Y. H. P., & Lynd, L. R. (2004). Toward an aggregated understanding of enzymatic hydrolysis of cellulose: Noncomplexed cellulase systems. Biotechnology and Bioengineering, 88(7), 797–824. Zhang, X., Liu, T., Sreekumar, T. V., Kumar, S., Moore, V. C., Hauge, R. H., et al. (2003). Poly(vinyl alcohol)/SWNT composite ﬁlm. Nano Letters, 3(9), 1285–1288. Zhu, S., Wu, Y., Chen, Q., Yu, Z., Wang, C., Jin, S., et al. (2006). Dissolution of cellulose with ionic liquids and its application: A mini-review. Green Chemistry, 8(4), 325–327.